CHEMICAL ENGINEERING TRANSACTIONS VOL. 50, 2016
A publication of
The Italian Association of Chemical Engineering Online at www.aidic.it/cet Guest Editors:Katharina Kohse-Höinghaus, Eliseo Ranzi
Copyright © 2016, AIDIC Servizi S.r.l., ISBN 978-88-95608-41-9; ISSN 2283-9216
Evaluation of Microstructure of Açaí Seeds Biomass Untreated and Treated with H2SO4 and NaOH by SEM, RDX
Johnatt A. R. Oliveiraa
, Rubens Maciel Filhob
a Nutrition College of Federal University of Pará, Augusto corrêa street, nº01, Belém, Pará, Brazil.
b Chemistry Engineering College of University of Campinas, Albert Einstein avenue, 500 – zip code: 13083-852, Campinas, São Paulo, Brazil.
The açaí seed is an abundant byproduct of açaí productive chain, Brazil`s northern region important fruit, especially in Pará and Amazonas states. However, it has been characterized as a hygienic-sanitary inconvenience to the region big cities, respectively Belém and Manaus. The use of this material to generate high added value products depends on better knowledge of its microstructure. This work aimed to analyse açaí seeds biomass using Scanning Electron Microscopy (SEM), X-Ray Diffraction (XRD) and Fourier Transform Infrared Spectroscopy (FTIR) in order to better understand its structural and chemical changes during treatment stages. For this purpose untreated, treated with H2SO4 and treated with H2SO4 and subsequently delignified with NaOH açaí seeds were used. SEM photomicrographs comparison showed that treatment with H2SO4 resulted in partial disruption of açaí seed structure, which became more evident after NaOH treatment. The crystallinity index for untreated açaí seeds was 47.05%, reducing after the treatments.
FTIR provided spectra in the region of 4000 to 400 cm-1. The used techniques allowed to observe significant structure changes caused by açaí seeds biomass treatment and provided information about microstructure of the untreated material.
Non-renewable fuels utilization is responsible for major environmental problems over time, such as global warming, climate change and health related problems. Along with global awareness about clean technology needs, a series of research efforts has emerged intending to propose viable alternatives economically and environmentally clean (Aransiola et al., 2014).
Around the world, lignocellulosic material is the most diverse and has shown great potential to ethanol fuel production (Rabelo et al., 2011). Besides its large availability as agroindustry residue, these materials are advantageously renewable (Singh and Trivedi, 2013).
In Brazil sugarcane is intensely used in ethanol production. Therefore its residues (bagasse and straw) utilization would be the first alternative to lignocellulosic ethanol production (Moraes et al, 2015). However Brazil`s north region does not produce sugarcane, impeding these material use for ethanol production. Still it has a strong açaí production agroindustry, regional fruit widely traded. Much of the post processed açaí (juice production) is disposed as seed, which is rich in lignocellulosic material (Oliveira, 2014).
Açaí seeds biomass utilization to produce fermentable sugars by chemical treatment (Oliveira et al., 2014) and enzymatic hydrolysis (Oliveira et al., 2015) are one of ways to obtain ethanol fuel. Besides being an excellent alternative on utilizing the large volume of this residue generated daily in northern Brazil big cities, such as Belém and Manaus (Oliveira, 2014).
Lignocellulosic biomass ethanol production demands good knowledge of the material structure used in the biotechnological transformation. During ethanol production steps a serie of modifications occur in the utilized biomass, changing its microstructures due to the transformation agents (Alnuami et al., 2014).
Please cite this article as: Oliveira J.A.R., Komesu A., Martins L.H., Maciel Filho R., 2016, Evaluation of microstrutcture of açaí seeds biomass untreated and treated with h2so4 and naoh by sem, rdx and ftir, Chemical Engineering Transactions, 50, 379-384 DOI: 10.3303/CET1650064
Good understanding of theses transformations enable the creation of enhanced methods and processes in the material utilization.
A few techniques already widely known in scientific community such as Scanning Electron Microscopy (SEM), X-Ray Diffraction (XRD) and Fourier Transform Infrared Spectroscopy (FTIR) can be used to deeply observe chemical and structural modifications in the transformed material, in the treatment and enzymatic hydrolysis steps (Balaji et al., 2015)
Thereby it is proposed to observe the chemical and microstructural behavior of açaí seed biomass before and after treatments, in order to obtain new information on this little known biomass, as well as the chemical treatment effects on açaí seed microstructure. Thus seeking more information about the potential of açaí seed for the production of ethanol.
2. Material and methods 2.1 Raw material
The açaí seeds were obtained in Belém - Pará - Brazil (01° 27' 21" S, 48° 30' 16" W) and were dried for 48h at 50°C in an air circulating oven and left for 48h at room temperature. The material was prepared according to Oliveira et al. (2015).
2.2. Treated and analyzed açaí seeds
Açaí seeds used on this work were: (1) - Raw açaí seed obtained according to item 2.1. (2) – Açaí seed treated with H2SO4 (10% of solid, 1% of acid for 60 minutes at 121°C), (3) - Açaí seed treated with H2SO4
(10% of solid, 1% of acid for 60 minutes at 121°C) and subsequently delignified (25% of solids, 1% of peroxide at 70°C during 60 minutes). Both H2SO4 treatment and sequential delignification were performed in retort at 120°C.
2.3 Imaging and spectroscopic techniques applied in açaí seeds characterization.
Untreated açaí seeds, treated with diluted H2SO4 and delignified, were analyzed using Scanning Electron Microscopy (SEM), X-Ray Diffraction (XRD) and Fourier Transform Infrared Spectroscopy (FTIR).
2.3.1. Scanning Electron Microscopy (SEM)
The micrographs were obtained using a Scanning Electron Microscope (SEM) with Energy Dispersive X-Ray Detector (EDX), model Leo 440i and EDS 6070, brand MEV/EDS: LEO Electron Microscopy/Oxford (Cambridge, England). Initial acceleration tension of 20kV and beam current of 100 pA were used.
2.3.2. X-Ray Diffraction (XRD)
Cellulose crystallinity index were determined through X-Ray Diffraction (XRD) to açaí seeds treated with diluted H2SO4 and delignified. Biomass crystallinity index (CrI) is defined as biomass crystalline material percentage and was calculated according to Segal et al., (1959).
2.3.3. Fourier Transform Infrared Spectroscopy (FTIR)
Fourier Transform Infrared Spectroscopy (FTIR) was used in chemical structures and functional groups identification in the evaluated samples based on Silva (2009) methodology.
3. Results and Discussions
3.1. Scanning Electron Microscopy (SEM) results
As observed in Figure 1(a) the material has some cut points and ruptures as a grinding process result.
Comparing Figures 1(a) and 1(b) a partial disorganization in the material structure is verified, due to the acid treatment, occasioning ruptures and fissures, which are related to lignin and carbohydrates chemical bonds disruption (Hendriks and Zeeman, 2009).
Great disorder of biomass structure was observed in Figure 1(c) after delignification of H2SO4 treated açaí seeds. It becomes visibly more porous and amorphous in comparison to untreated material (a) or H2SO4
treated (b). As also verified by Zúñiga (2010) this material heterogeneity is a complicating factor to more efficient MEV biomass structure evaluation. In Figure 1 (a, b and c) are presented photomicrographies of treated and untreated açaí seeds.
3.2. X-Ray Diffraction (XRD) crystallinity index results
In Figure 2 is shown X-Ray Diffraction calibration curves used to calculate the crystallinity index observed in Table 1. Studied samples analysis showed açaí seeds crystallinity index of 47.05%, smaller then described by Rodriguez-zuñiga (2010) to sugarcane bagasse (58.18%) and by Ayala (2012) to sugarcane straw (49.01%).
Crystallinity index after acid treatment (in analyzed conditions) reduced only 11% in comparison to untreated material. treated and subsequently delignified material displayed 64% reduction in comparison to raw material.
As showed in Table 1, crystallinity index fixed to yield basis was 41.64% to H2SO4 treated material and
17.01% after delignification. Similar results were founded by Samuel et al. (2012) who noted that diluted H2SO4 treatment promoted 12% reduction in switchgrass biomass crystallinity. To the treated and subsequently delignified material showed 64% reduction in comparison to untreated material. As shown in Table 1, crystallinity index corrected to yield basis is 41.64% to acid treated material and 17.01% after delignification.
Figure 1. Untreated açaí seed (a), post diluted H2SO4 treatment (b) and post diluted H2SO4 and sub sequentially delignified (c) photomicrographs.
Thereby, it is possible to claim the delignification was highly effective in reducing açaí seed crystallinity, which happens most likely due to lignin and hemicellulose removal than for cellulose I to cellulose II conversion. The evidence of this standpoint is in the diffractogram peaks in untreated material and treated and subsequently delignified material, it shows 2θ peaks in 16° (002 plan) and 18° (101) which corresponds to cellulose I (Terinte et al., 2011). Therefore it is not possible to claim the reduction in crystallinity is result of cellulose I to cellulose II conversion.
Ben Sghaier et al. (2012) treated American Agave fibers and observed NaOH concentrations above 5% cause crystallinity reduction of cellulose fibers around 15%, which was caused by fiber swelling after alkaline agent penetration.
The same authors claim that, during treatment, cellulose fibers are rearranged from cellulose I (parallel aligned chains) to cellulose II (anti-parallel). What was not observed to the açaí seed mercerizing probably as result of the alkaline agent low concentration. Previous research report cellulose I to cellulose II transformation occurs in NaOH concentrations above 6% (Moigne and Navard, 2010).
Figure 2. X-Ray Diffraction calibration curves used to calculate the crystallinity index
Table 1. Crystallinity index (CrI) obtained to untreated açaí seeds, treated with diluted H2SO4 and treated with acid and subsequently delignified.
Açaí seeds Crystallinity
Untreated 47,05 - -
Treated with H2SO4 dilute 64,07 65 41,64 Treated with H2SO4 and delignified 71,35 23,85 17,01 3.3. Fourier Transform Infrared Spectroscopy (FTIR) results
FTIR was used to investigate açaí seeds physical structure and functional groups. Thereby, in Figure 3, it is possible to verify FTIR spectra in the 4000 to 400 cm-1 range in the present work.
The spectra main characteristics were assigned to presence of lignin, hemicellulose and cellulose, natural fibers typical components. In this kind of material, modified or not, is common to observe a 3100-3500 cm-1 band appearing, a broadband, associated to the O-H group axial deformation. In this way untreated açaí seed fibers spectra was characterized by a 3411 cm-1 band, which refers to the OH groups vibrational stretch (Merlini, 2011). To the treated or delignified analysed material a drastic decrease in absorptivity is observed, due to cellulose removal during treatment.
Figure 3. FTIR spectra to untreated açaí seed (raw material), treated and treated and subsequently delignified.
Each of the following numbers points to identified and discussed peaks: (1) 3411; (2) 2921; (3) 2875; (4) 2852; (5) 1743 (6) 1629 (7)1517 (8)1445 (9)1378 (10) 1321; (11)1245; (12) 1160; (13) 128; (14)1099; (15) 1010; (16)1060; (17) 937; (18)871; (19) 804.
The 2894-2950 cm-1 can be assigned to the C-H stretching, such as observed by Khalil et al. (2001). On this band the 2921, 2875 and 2852 cm-1 peaks were observed, which are related to the C-H aliphatic stretching of the methyl (CH3) and methylene (CH2) groups (Sinha and Rout, 2008). As pointed by Kim et al. (2003) the bands intensity related to characteristic lignin peaks (1502-1600 cm-1 range) was bigger to the acid treated material and much bigger to the treated and subsequently delignified material, which proves the lignin removal treatments effect.
The 1742 cm-1 peak in untreated material is characteristic of the carbonyl (C=O) stretching, assigned to the hemicellulose (Owen and Thomas, 1989) in açaí seeds and which presented lower intensity to the treated and delignified material, showing hemicellulose removal in the treatment process. The 1629 cm-1 peak represent residual water in all presented spectra (Nacos et al., 2006; Troedec et al., 2008).
Intensity difference between 1510 and 1600 cm-1 bands can be used to distinguish conifer lignin (high content of guaiacyl groups) from broadleaf lignin (higher content of syringyl) (Owen and Thomas, 1989; Colom et al., 2003; Fengel and Wegener, 2003). Comparing the açaí seed existing bands, it is possible to observe the 1600 cm-1 band presents the highest intensity, which indicates the analysed material lignin has higher content of sygingyl units.
According to the literature, the 1517, 1445, 1378 and 1321 cm-1 peaks are related to the C-C bon in the aromatic, methyl group asymmetric deformation, C-H stretching in polysaccharides and hydroxyl angular deformation (-OH) in the lignin aromatic ring (Nacos et al., 2006; Troedec et al., 2008).
The 1245 cm-1 peak band is related to acetyl group stretching of hemicellulose, however lignin also contributes to this band formation. The 1160, 1128 and 1099 cm-1 peaks band indicates C-O-C asymmetric stretching in cellulose and hemicellulose.
The 1010, 1060 and 1164 cm-1 peaks (not showed in Figure 3) are characteristic of the C-O, C=C and C-C-O groups stretching of cellulose, hemicellulose and lignin (Sills et al., 2012). The peaks absorptivity values in acid treated material showed higher values than the untreated and delignified ones. It has happened due to hemicellulose removal during acid treatment, showing lignin’s structure in hemicellulose absence. It is possible to verify drastically reduced absorptivity after delignification, which exhibits lower values than the untreated material and H2SO4 treated ones.
Finally, the 937, 871 and 804 cm-1 peaks, observed in all materials, could be assigned to the C-O-C stretching in the β-glucosides bonds (Ciolacu et al., 2011).
It was possible to conclude the used tools to untreated and treated açaí seed microstructure evaluation allowed a better understanding of the material and the treatment effects on the material modification point of view. SEM imaging showed more effective lignocellulosic material disruption after H2SO4 and delignification treatment, which also showed the lowest crystallinity after lignin and hemicellulose removal. Whereas FTIR allowed to verify important chemical alterations in the analysed treated materials.
Alnuami. W., Buthainah. A., Etti. C. J., Jassim. L.I., Gomes. G. A., 2014. Evaluation of Different Materials for Biodiesel Production. International Journal of Innovative Technology and Exploring Engineering, 3 1-8.
Aransiola, E.F., Ojumu T.V., Oyekola, O.O., Madzimbamuto, T.F., Ikhu-Omoregbe, D.I.O., 2014, A review of current technology for biodiesel production: State of the art. Biomass and bioenergy, 61, 267-297.
Ayala, O.L., 2012, Pre-treatment evaluation for enzymatic hydrolysis of straw sugarcane considering the ethane production. Thesis of Doctorate, UNICAMP, Campinas, São Paulo, 120 pages.
Balaji, A., Karthikeyan. B., Sundar Raj. C. 2015, Bagasse Fiber – The Future Biocomposite Material: A Review, International Journal of ChemTech Research, 7, 223-233.
Ben sghaier, A.O.; Chaabouni, Y.; Msahli, S.; Sakli, F., 2012, Morphological and crystalline characterization of NaOH and NaOCl treated. Agave americana L. fiber. Industrial Crops and Products, 36, 257–266.
Ciolacu, D.; Ciolacu, F.; Popa, V. I., 2011, Amorphous cellulose -structure and characterization. Cellulose Chemistry and Technology, 45, 13-21.
Colom, X.; Carrillo, F.; Nogues, F.; Garriga, P., 2003, Structural analysis of photodegraded wood by means of ftir spectroscopy. Polymer Degradation and Stability, 80, 543-549.
Fengel, D.; Wegener, G., 2003, Wood: Chemistry, ultrastructure, reactions. Germany: KesselVerlag, Remagen. 611p.
Hendriks. A.T.W.M., Zeeman. G., 2009, Pretreatments to enhance the digestibility of lignocellulosic biomass.
Bioresource Technology, 100, 10–18.
Khalil, H.P.A.; Ismail, H. Rozman, H.D.; Ahmad, M.N., 2001, The effect of acetylation on interfacial shear strength between plant fiber and various matrices. European Polymer Journal., 5, p.1037-1045.
Kim, T.H.; Kim, J.S.; Sunwoo, C. Lee, Y.Y., 2003, Pretreatment of corn stover by aqueous ammonia.
Bioresource Technology, 90, 39-47.
Merlini, C. 2011Experimental analysis of composite polyurethane derived from castor oil and banana fibers, Dissertation of master of Sciences and materials Engineering, Federal University of Santa Catarina, Santa Catarina, 2011.
Moigne N.L.; Navard, P., 2010, Dissolution mechanism of wood cellulose fibres in NaOH–water. Cellulose, 17, 31–45.
Moraes. B.S., Zaiat. M., Bonomi.A., 2015, Anaerobic digestion of vinasse from sugarcane ethanol production in Brazil: Challenges and perspectives. Renewable and Sustainable Energy Reviews, 44, 888–903.
Nacos. M., Katapodis. P., Pappas. C., Daferera. D., Tarantilis. P. A., Christakopoulos. P., Polissiou. M., 2006, Xylan-A source of biologically active acidic oligosaccharides. Carbohyd. Polymers, 1, 126-134.
Oliveira. J.A.R., Komesu. A., Maciel Filho. R., 2014, Hydrothermal Pretreatment for Enhancing Enzymatic Hydrolysis of Seeds of Açaí (Euterpe oleracea) and Sugar Recovery. Chemical engineering transactions, 37, 787-792.
Oliveira. J.A.R., Martins. L.H.S., Komesu. A., Maciel Filho. R., 2015. Evaluation of Alkaline Delignification (NaOH) of Açaí Seeds (Eutherpe Oleracea) treated with H2SO4 Dilute and Effect on Enzymatic Hydrolysis. Chemical engineering transactions, 43, 499-504.
Owen. N. L., Thoma.S, D. W., 1989, Infrared studies of hard and soft woods. Applied Spectroscopy, 43, 451- 455.
Rabelo S.C., Carrere H., Maciel Filho R., Costa A.C., 2011, Production of bioethanol, methane and heat from sugarcane bagasse in a biorefinery concept, Bioresource Technology, 102, 7887-7895.
Samuel. R., Pu. Y., Raman. B., Ragauskas. A., 2010, Structural characterizations and comparison of switchgrass lignin before and after dilute acid pretreatment. Applied Biochemistry and Biotechnology, 162, 62-74.
Segal. L.,Creely, J. J., Martin. A. E., Conrad. C. M., An empirical method for estimating the degree of crystallinity of native cellulose using the x-ray diffractometer. Textile Research Journal, 29, 786-764, 1959.
Sills, D.L.; Gossett, J.M., 2012, Using FTIR to predict saccharification from enzymatic hydrolysis of alkali pretreated biomasses. Biotechnol Bioeng, 109, 353–62.
Silva, V.F.N., 2009, Studies pretreatment and enzymatic saccharification stages in agroindustrial residues as cellulosic ethanol obtaining process. Dissertation of master’s degree (Master in Sciences), University of São Paulo. 116 pages.
Singh. D.P., Trivedi. R.K., 2013, Biofuel from Wastes an Economic and Environmentally Feasible Resource.
Energy Procedia, 54, 634–641.
Sinha. E., Rout. S.K.,2008, Influence off fibre-surface treatment on structural, thermal and mechanical properties of jute. Journal of Materials Science, 43, 2590-2601.
Terinte. N., Ibbet. R., Schuster. K.C., 2011, Overview on native cellulose and microcrystalline cellulose I structure studied by x-ray diffraction (WAXD): comparison between measurement techniques. Lezinger Berichte, 89, 118-131.
Troedec, M., Sedan, D., PeyratouT, C., 2008, Bonnet, J., Smith, A., Guinebretiere, R., Gloaguen, V., Krausz, P. Influence of various chemical treatments on the composition and structure of hemp fibers. Composites Part A-Applied Science And Manufacturing. 3, 514-522.
Zúñiga, U. F. R., 2010, Bioprocess development for production of specific cellulases in the production chain of second-generation ethanol. Thesis of doctorate – University of São Paulo, 228 pages.